|Year : | Volume
| Issue : | Page :
|Surface roughness in nanoparticle resin composites subjected to two polishing systems: An in vitro comparative study
Giovanna Gisella Ramírez-Vargas1, Marysela I Ladera-Castañeda2, Carlos López-Gurreonero3, Alberto Cornejo-Pinto1, Hernán Cachay-Criado4, Luis Adolfo Cervantes-Ganoza5, César Félix Cayo-Rojas4
1 Universidad Nacional Federico Villarreal, Postgraduate School, “Grupo de Investigación Salud y Bienestar Global”, Lima, Peru
2 Universidad Nacional Federico Villarreal, Postgraduate School, “Grupo de Investigación Salud y Bienestar Global”, Lima, Peru; Universidad Privada San Juan Bautista, School of Stomatology, Lima and Ica, Peru
3 Universidad Científica del Sur, School of Stomatology, Lima, Peru
4 Universidad Privada San Juan Bautista, School of Stomatology, Lima and Ica, Peru
5 Universidad Inca Garcilaso de la Vega, Faculty of Stomatology, Lima, Peru
|Date of Submission||25-Sep-2021|
|Date of Decision||29-Nov-2021|
|Date of Acceptance||05-Dec-2021|
|Date of Web Publication||09-Nov-2022|
César Félix Cayo-Rojas,
Universidad Privada San Juan Bautista, School of Stomatology, Av. Jose Antonio Lavalle s/n; Chorrillos. Lima 15066
Source of Support: None, Conflict of Interest: None
| Abstract|| |
Aim: The surface roughness of dental restorations can decrease resin durability, since it leads to its deterioration, color variation, and loss of gloss. Therefore, the aim was to assess the surface roughness of nanoparticle resin composites, subjected to two different polishing systems. Materials and Methods: This longitudinal in vitro experimental study consisted of 32 resin specimens made according to ISO 4049-2019 and divided equally into four groups: A1: Palfique LX5 / Sof-Lex, A2: Palfique LX5 / Super Snap, B1: Filtek Z350 XT / Sof-Lex, and B2: Filtek Z350 XT / Super Snap. The samples were stored in distilled water at 37°C for 24 h. Surface roughness was measured with a digital roughness tester, both before and after the polishing procedure. The data were analyzed with the Student’s t-test for related samples, and with the inter-subject ANOVA test with two factors; considering significance at P < 0.05. Results: The surface roughness of Palfique LX5 resin with the Sof-lex system was 0.330 (CI: 0.282–0.378 µm) and 0.170 (CI: 0.087–0.253 µm) before and after polishing, respectively. With the Super Snap system, values of 0.448 (CI: 0.346–0.549 µm) and 0.206 (CI: 0.130–0.282 µm) were obtained before and after polishing, respectively. For the Filtek Z350 XT resin, the surface roughness obtained with the Sof-lex system was 0.353 (CI: 0.278–0.427 µm) and 0.134 (CI: 0.095–0.172 µm) before and after polishing, respectively. With the Super Snap system, values of 0.334 (CI: 0.247–0.421 µm) and 0.171 (CI: 0.122–0.221 µm) were obtained before and after polishing, respectively. Surface roughness did not show significant differences in all groups assessed both before (P = 0.068) and after (P = 0.335) polishing. However, before and after the application of the polishing systems, all groups significantly decreased their surface roughness (P < 0.05). Further, when comparing this decrease among all groups, no significant differences were observed (P = 0.437). Conclusion: The surface roughness of the Filtek Z350 XT and Palfique LX5 nanoparticle resin composites showed no significant differences when using the Sof-lex and Super Snap polishing systems. However, both polishing systems significantly decreased the surface roughness of the nanoparticulated resins, with this decrease being similar in all groups.
Keywords: Comparative study, dental materials, dental polishing, dentistry, resin composite, surface roughness
|How to cite this URL:|
Ramírez-Vargas GG, Ladera-Castañeda MI, López-Gurreonero C, Cornejo-Pinto A, Cachay-Criado H, Cervantes-Ganoza LA, Cayo-Rojas CF. Surface roughness in nanoparticle resin composites subjected to two polishing systems: An in vitro comparative study. J Int Soc Prevent Communit Dent [Epub ahead of print] [cited 2022 Nov 30]. Available from: https://www.jispcd.org/preprintarticle.asp?id=360630
| Introduction|| |
Aesthetic dentistry today has made significant advances in restorative materials and their application techniques, which have allowed dentists to improve their treatments in terms of aesthetics and functionality.,, With the contribution of nanotechnology, it has been possible to develop resin composites that include in their structure a filling of nanoparticles and nanocluster agglomerates, which are of vital importance since the smaller they are, the better the wear resistance, gloss retention, and polishing capability. In addition, they are currently considered to be the biomaterials with the highest aesthetic demand, since they perfectly reproduce the color, texture, and translucency of teeth, as well as have been exhibiting ideal clinical performance over the years.,
The presence of roughness on the surface of dental restorations can reduce their durability, since it leads to the deterioration of the resin, color variation, and loss of brightness.,In vitro studies have evaluated the surface roughness threshold of resin composites, reporting that the average roughness value higher than 0.2 microns can cause retention and a substantial increase of bacterial plaque; thus, obtaining a smooth surface reduces the risk of plaque accumulation and helps to avoid pigmentations that alter the natural appearance of restorations.,, For this reason, finishing and polishing procedures are considered of vital importance in the dental restoration process, since they allow not only the elimination of rough surfaces, but also the elimination of the oxygen-inhibited layer, achieving surfaces with ideal aesthetics that last over time.,
Resin composites containing nanoparticles are less susceptible to particle detachment caused by contact with the abrasive material of polishing systems, favoring the reduction of surface roughness.,, In this regard, Palfique LX5 resin, whose filler is based on nanoparticles with a size ranging from 0.1 to 0.3µm, has 71% of its volume filled with silica-zirconium dioxide and composite, which gives it a lower shrinkage in the polymerization process and good wear resistance, without losing the conditions to obtain an optimum polish and shine. On the other hand, the Z350 XT resin has zirconium and silica particles or nanoclusters with a range of 5 to 20 nm, which gives it good wear resistance and excellent gloss retention in polishing.
Currently, there are different polishing systems for the finishing of resin composites, which can generate surfaces with a certain degree of roughness, either due to the number of polishing steps used or due to the physical characteristics of the resin composites themselves. Therefore, it is important that in clinical procedures, the dental professional can differentiate and select the polishing treatment that best suits the resin composite used, taking into consideration: the polishing system, the particle size of the resin composite, its physical and mechanical properties, and the consistent scientific evidence that allows an optimal protocol for a functional and esthetic restoration with the greatest possible longevity.,
The Sof-Lex 3M and Super Snap polishing systems used in this study are currently considered as good polishing alternatives, since they are applied through a multistep system consisting of four flexible disks impregnated with aluminum oxide and, in some cases, with silicon carbide, which allows a better adaptation to the restoration surface, while performing a selective sequence of abrasion to obtain a smoother and more homogeneous surface.,
In view of what has been cited earlier, the objective of this study was to evaluate the surface roughness of resin composites with Palfique LX5 and Filtek Z350 XT nanoparticles subjected to two polishing systems: Sof-Lex 3M and Super Snap. This study considered the CRIS Guidelines (Checklist for Reporting In-vitro Studies).
| Materials and Methods|| |
Type of study and delimitation
This experimental in vitro, longitudinal, and prospective study was carried out at the Postgraduate School of the Universidad Nacional Federico Villarreal and at the High Technology Laboratory Certificate (ISO / IEC Standard: 17025), Lima, Peru, in the months of October to December 2020.
Sample calculation and selection
Thirty-two resin specimens were standardized and fabricated, which were equally distributed in four groups. The sample size per group was eight resin composite specimens (n = 8), and it was calculated based on data obtained in a previous pilot study, where the mean comparison formula was applied considering a significance level (α) = 0.05 and a statistical power (1-β) = 0.80, with variances S12 = 0.017 and S22 = 0.019 and a mean difference equal to 0.2 µm. The sample units were distributed, in a simple random manner without replacement, in four groups according to the treatment used. For this, the method used was double blinded, since the laboratory assistant who performed the random distribution and the statistician who processed the results were unaware of the assignment of the samples to each group [Figure 1].
The variables included were: type of nanoparticulated resin composite, type of polishing system, and surface roughness.
Sample characteristics and preparation
Specimens of resin composites with Filtek Z350 XT nanoparticles (3M ESPE, St. Paul, MN, USA) and Palfique LX5 (Tokuyama Dental Corporation, Taitō-Ku, Tokyo, Japan), both color A2, were used for this study [Figure 2]. These were prepared with standardized molds of 6 mm diameter and 4 mm depth, according to ISO 4949-2019. Molds for the resin composite specimens were placed on a 1-mm-thick microscope slide, using the same procedure to light cure the last layer of the specimen, ensuring that the upper and lower surfaces were parallel. The resin composite layers were light-cured from the upper part of the mold with an LED (light emitting diode) lamp (EliparTM Deep Cure-L, 3M ESPE, St. Paul, MN, USA) at a light intensity of 1200 mW/cm2 for 20 sec, verifying it with a radiometer (Litex 682, Dentamerica, Industry, CA, USA). Once the specimen was ready, glycerin was applied on the surface and final light curing was performed for 20 sec in order to avoid the formation of the oxygen-inhibited layer [Figure 3].
|Figure 2: (A) Materials and instruments used. (B) Compaction of resin composite inside the stainless-steel mold|
Click here to view
|Figure 3: (A) Light curing of the resin composite. (B) Resin specimen according to ISO:4049-2019|
Click here to view
Surface roughness test
Once the 32 resin specimens were obtained, the surface roughness was measured before the polishing procedure was performed. After that, they were stored in an oven at 37°C for 24 h. The next day, all the specimen surfaces were polished according to the type of treatment assigned to each group [Figure 4] and [Figure 5]. Subsequently, the surface roughness was measured again after polishing. Each resin specimen was measured with a digital roughness tester (SRT-6200, Huatec, Beijing, Haidian, China). The surface roughness value on each resin specimen was determined with the average in microns of the measurements in four different areas of the surface [Figure 6].
|Figure 6: (A) Surface roughness measurement. (B) HUATEC SRT-6200 roughness tester|
Click here to view
The data collected were recorded in a Microsoft Excel 2019 file and subsequently imported for statistical analysis by using SPSS (Statistical Package for the Social Sciences Inc. IBM, NY, USA) version 24.0. For descriptive analysis, measures of central tendency and dispersion, such as mean and standard deviation, were used. For the inferential analysis, the Shapiro-Wilk test was used to evaluate whether the data had a normal distribution, the Levene homoscedasticity test was used to evaluate the homogeneity of variances, and the Wald-Wolfowitz test was used to analyze the randomness of the sample units based on the mean. When verifying that the three statistical assumptions were met, it was decided to use the parametric Student’s t-test for related samples, and also the two-factor inter-subject ANOVA test. In all comparisons, a P < 0.05 was considered for significant differences.
| Results|| |
The surface roughness obtained on Palfique LX5 resin composite with the Sof-lex system was 0.330 (CI: 0.282–0.378 µm) and 0.170 (CI: 0.087–0.253 µm) before and after polishing, respectively. Likewise, values of 0.448 (CI: 0.346–0.549 µm) before and 0.206 (CI: 0.130–0.282 µm) after the Super Snap polishing system were obtained [Table 1].
|Table 1: Descriptive values for the surface roughness of Palfique LX5 resin composite before and after applying different polishing systems|
Click here to view
For the Filtek Z350 XT resin composite, the surface roughness obtained with the Sof-lex system was 0.353 (CI: 0.278–0.427 µm) and 0.134 (CI: 0.095–0.172 µm) before and after polishing, respectively. Likewise, such resin composite obtained the values of 0.334 (CI: 0.247–0.421 µm) and 0.171 (CI: 0.122–0.221 µm) before and after being subjected to the Super Snap system, respectively [Table 2].
|Table 2: Descriptive values for the surface roughness of Filtek Z350 XT resin composite before and after applying different polishing systems|
Click here to view
Surface roughness had similar values in all groups of resin composites before the application of different polishing systems, showing that there were no significant differences (P = 0.068) [Table 3] and [Graph 1].
|Table 3: Comparison of surface roughness between resin composite groups before applying different polishing systems|
Click here to view
|Graph 1: Comparison of surface roughness with 95% confidence interval between groups of resin composites before applying the different polishing systems|
Click here to view
When comparing the surface roughness between the resin composite groups after applying the different polishing systems, no significant differences were observed (P = 0.335) [Table 4] and [Graph 2].
|Table 4: Comparison of surface roughness between resin composite groups after applying different polishing systems|
Click here to view
|Graph 2: Comparison of average surface roughness with 95% confidence interval between resin composite groups after applying different polishing systems|
Click here to view
When performing the individual analysis between the resin composite groups before and after the application of the different polishing systems, it could be observed that all the evaluated groups significantly reduced their surface roughness values (P < 0.05) [Table 5].
|Table 5: Comparison of surface roughness between Palfique LX5 and Filtek Z350 XT resin composites before and after applying different polishing systems|
Click here to view
When comparing the differences in the averages between before (Ⴟi) and after (Ⴟf) applying the different polishing systems, there were no statistically significant differences between the Palfique LX5 and Filtek Z350 XT resin composites (p=0.437) [Table 6] and [Graph 3].
|Table 6: Comparison of surface roughness variation between resin composite groups, before and after applying different polishing systems|
Click here to view
|Graph 3: Comparison of average difference in surface roughness values between resin composite groups before and after application of polishing systems|
Click here to view
| Discussion|| |
The purpose of this in vitro study was to evaluate the surface roughness of nanoparticle resin composites subjected to two polishing systems. The resin composites used in this study were Palfique LX5 and Filtek Z350 XT with Sof-Lex and Super Snap polishing systems. After analyzing the results, it was found that when comparing the differences in surface roughness values, before and after being subjected to two polishing systems, no significant differences were observed between the resin composites used. This may be because resin composites containing nanoparticle fillers are less susceptible to particle shedding when they come in contact with the abrasive material of the polishing disks, resulting in less surface irregularity. This is consistent with that reported by Dias et al, who concluded that nanoparticle composite resins showed higher performance, since they are composed of agglomerates of zirconium-silica particles (nanoclusters) with a low compact nanometer-sized filler and a higher percentage of inorganic filler, which favors a lower detachment of these particles during polishing, thus generating a surface with fewer defects and better polish retention. However, it should be noted that in the present investigation, when evaluating the effectiveness of the Sof-lex and Super Snap polishing systems, they significantly reduced the surface roughness of the nanoparticulated resin composites Palfique LX5 and Filtek Z350 XT, probably because it was achieved by applying a four-step sequence of disks impregnated with aluminum oxide abrasive particles, from coarse to fine grain.
The preparation of the resin composite specimens was performed according to ISO Standard 4049-2019, and the polishing procedure was carried out following the manufacturer’s indications. In addition, the sample was kept in an oven with distilled water to simulate the humid environment of the oral cavity and thus allow the final polymerization process. In addition, the application of glycerin on the surface of all resin composite specimens prior to light curing the last layer was included as part of the procedure, in order to avoid the formation of the oxygen-inhibited layer that would generate water or saliva absorption and subsequent discoloration of the resin composite. Therefore, Marigo et al. recommended the use of glycerin before light curing the last layer of resin, since it forms a physical barrier that optimizes the conditions of the polymerization process by acting as an inhibitor of atmospheric oxygen, and it also converts the highly reactive radicals of the surface into relatively stable hydroperoxides, allowing to obtain a better quality of light curing in the outermost layer of resin composites.
In this study, the resin composites Palfique LX5 and Z350 XT when polished with the Sof-Lex system presented minimum surface roughness values of 0.080 µm and 0.070 µm, respectively, whereas with the Super Snap system they presented minimum surface roughness values of 0.070 µm for both. These values are in agreement with the surface quality standard ISO 1302:2002, since this standard considers surface roughness between 0.0025 µm and 0.80 µm as acceptable. Further, the values obtained in this study are in agreement with those obtained by Midobuche et al, who evaluated the surface roughness of Sof-Lex polishing systems on aesthetic nanoparticle resins, obtaining surface roughness values below 1 µm, which corresponds to clinically acceptable parameters.
Regarding the polishing systems used in this study, these consist of four paper disks coated with aluminum oxide ranging from coarse to superfine grain, with the difference that the Super Snap disks are also coated with silicon carbide and have a homogeneous surface. On the other hand, Sof-Lex disks have a metal ring in the central part, which offers greater flexibility and capacity to adapt to different surfaces, allowing uniform wear and a lower level of abrasiveness, resulting in both polishing systems being effective in significantly reducing the surface roughness of the resin composites used in this study. This was in agreement with the study by Balbina et al, who reported that using abrasive disks impregnated with aluminum oxide presented a better performance in reducing the surface roughness of resin composites. Likewise, a study by Yucci compared the surface roughness of composite resins under the application of different polishing systems and concluded that the surface roughness was influenced by the particle size, hardness and the amount of resin filler, as well as the flexibility of the material used for polishing, with this being reinforced by the study of Alfawaz, who reported that the surface roughness varies according to the polishing system and resin composite used.
The decision to study nanoparticle resin composites and the polishing systems that act on them was due to the importance and influence that the polishing procedure has on the durability of the restorative treatment. There are several polishing systems in the dental field with different composition of abrasive material that influence the clinical performance of the resin composite, so in this study the most known and recommended systems by different authors were tested.,
The present study is important because, in view of the results obtained, the nanoparticulated resin composites present better surface quality when a Sof-lex or Super Snap polishing system is applied to them, due to the fact that the nanoparticulated resin composites have filler particles of less than one micron in their composition, resulting in a high wear resistance that significantly reduces the probability of creating grooves and irregularities on the surface, with an excellent polish and high gloss, facilitating the longevity of the resin composite both aesthetically and functionally.,,,,
As a limitation of the present study, it is recognized that the results obtained cannot be extrapolated to the clinical field, since the design of this research was in vitro. Therefore, it is recommended that randomized clinical trials related to the proposed objective be performed. In addition, it is recommended to develop comparative studies with the same proposed research design, including polishing systems of one or more steps, Bulk Fill type resin composites, as well as controlling the variable of glycerin application before the last light-curing process.
| Conclusion|| |
In summary, considering the limitations of the present in vitro study, the surface roughness of the Filtek Z350 XT and Palfique LX5 nanoparticulate resin composites showed no significant differences when using the Sof-lex and Super Snap polishing systems. However, both polishing systems significantly decreased the surface roughness of the nanoparticulated resin composites, with this decrease being similar in all groups.
The authors thank the Postgraduate School of the Universidad Nacional Federico Villarreal, Lima, Peru, for their constant support in the preparation of this article.
Financial support and sponsorship
Conflicts of interest
None to declare.
They conceived the research idea (GGRV), elaborated the article (GGRV, MILC, LACG, CFCR), collected, tabulated the information (GGRV, CLG), carried out the bibliographic search (MILC, ACP, CLG), interpreted the statistical results (CFCR), helped in the development of the discussion (GGRV, HCC, ACP, CFCR), and performed the critical review of the article (GGRV, HCC, LACG, CFCR). All authors approved the final version of the article.
Ethical policy and institutional review board statement
This project is exempted from ethical approval due to it being an experimental in vitro study.
Patient declaration of consent
Data availability statement
The data that support the study results are available from the author (Dra. Giovanna Ramírez-Vargas, e-mail: [email protected]) on request.
| References|| |
Cayo C, Llancari L, Mendoza R, Cervantes L Marginal filling and adhesive resistance of bulk fill resin applying 18% edta gel compared with 37% phosphoric acid gel in vitro
dental conditioning. J Oral Res 2019;8:228-35.
Blatz MB, Chiche G, Bahat O, Roblee R, Coachman C, Heymann HO Evolution of aesthetic dentistry. J Dent Res 2019;98:1294-304.
Cayo C, Carrillo A Marginal sealing applying sodium hypochlorite versus phosphoric acid as dental conditioner. Rev Cubana Estomatol 2020;57:e2872.
Moura P, Azevedo S, Dutra B, Vieira I, Alves G Impact of a novel polishing method on the surface roughness and micromorphology of nanofilled and microhybrid composite resins. Revista Portuguesa de Estomatologia, Medicina Dentária e Cirurgia Maxilofacial 2015;56:18-24.
Alzraikat H, Burrow MF, Maghaireh GA, Taha NA Nanofilled resin composite properties and clinical performance: A review. Oper Dent 2018;43:E173-90.
Wheeler J, Deb S, Millar BJ Evaluation of the effects of polishing systems on surface roughness and morphology of dental composite resin. Br Dent J 2020;228:527-32.
Lopes IAD, Monteiro PJVC, Mendes JJB, Gonçalves JMR, Caldeira FJF The effect of different finishing and polishing techniques on surface roughness and gloss of two nanocomposites. Saudi Dent J 2018;30:197-207.
Hyun HK, Salehi S, Ferracane JL Biofilm formation affects surface properties of novel bioactive glass-containing composites. Dent Mater 2015;31:1599-608.
Bayrak GD, Sandalli N, Selvi-Kuvvetli S, Topcuoglu N, Kulekci G Effect of two different polishing systems on fluoride release, surface roughness and bacterial adhesion of newly developed restorative materials. J Esthet Restor Dent 2017;29:424-34.
Bollen CM, Lambrechts P, Quirynen M Comparison of surface roughness of oral hard materials to the threshold surface roughness for bacterial plaque retention: A review of the literature. Dent Mater 1997;13:258-69.
Sang EJ, Song JS, Chung SH, Jin BH, Hyun HK Influence of a new polishing system on changes in gloss and surface roughness of resin composites after polishing and brushing. Dent Mater J 2021;40:727-35.
Daud A, Adams AJ, Shawkat A, Gray G, Wilson NHF, Lynch CD, et al
. Effects of toothbrushing on surface characteristics of microhybrid and nanofilled resin composites following different finishing and polishing procedures. J Dent 2020;99:103376.
Resin-based Dental Restorative Material PalfiqueTM LX5. Tokuyama Dental Corporation. Technical profile of the product. Available from: http://www.tokuyama-dental.com/tdc/pdf/instructionmanual/PALFIQUE_LX5_IFU.pdf
. [Last accessed on 2021 May 14].
Filtek™Z350XT Universal Restorative System. Technical profile of the product Available from: https://pdf4pro.com/view/filtek-z350-xt-technical-product-profile-350664.html
. [Last accessed on 2021 May 16].
Jaramillo-Cartagena R, López-Galeano EJ, Latorre-Correa F, Agudelo-Suárez AA Effect of polishing systems on the surface roughness of nano-hybrid and nano-filling composite resins: A systematic review. Dent J (Basel) 2021;9:1-17.
Tosco V, Monterubbianesi R, Orilisi G, Procaccini M, Grandini S, Putignano A, et al
. Effect of four different finishing and polishing systems on resin composites: Roughness surface and gloss retention evaluations. Minerva Stomatol 2020;69:207-14.
3M ESPE Dental Products. Sof-Lex. Product Technical Profile Finishing and Polishing Systems. Available from: https://multimedia.3m.com/mws/media/180294O/sof-lextm-technical-profile.pdf
. [Last accessed on 2021 May 12].
SHOFU INC. Super Snap. Technical Profile of the Product. Finishing and Polishing System. Available from: https://www.shofu.com/wp-content/uploads/Super-Snap-IFU-US.pdf
. [Last accessed on 2021 May 14].
Krithikadatta J, Gopikrishna V, Datta M Cris guidelines (checklist for reporting in-vitro studies): A concept note on the need for standardized guidelines for improving quality and transparency in reporting in-vitro studies in experimental dental research. J Conserv Dent 2014;17:301-4.
ISO 4049:2019-Dentistry-Polymer-based Restorative Materials. Available from: https://www.iso.org/standard/67596.html
. [Last accessed on 2021 Jul 9].
Dias LI, Cardoso MP, Baltazar MJ, Rua GJ, Fernandes CF The effect of different finishing and polishing techniques on Surface roughness and gloss of two nanocomposites. Saudi Dent J 2019;30:197-207.
Marigo L, Nocca G, Fiorenzano G, Callà C, Castagnola R, Cordaro M, et al
. Influences of different air-inhibition coatings on monomer release, microhardness, and color stability of two composite materials. Biomed Res Int 2019;2019:4240264.
ISO 1302:2002. Geometrical Product Specifications (GPS). Indication of Surface Texture in Technical Product Documentation. Available from: https://www.iso.org/obp/ui/es/#iso:std:iso:1302:en
. [Last accessed on 2021 Jul 9].
Midobuche PEO, Zermeño LMT, Guízar MJM, et al
. Determinación de la calidad de pulido de resinas de nanorrelleno empleando un microscopio de fuerza atómica. Rev ADM 2016;73:255-62.
Balbina K, Polyakova M, Sokhova I, Doroshina V, Arakelyan M, Novozhilova N The effect of finishing and polishing sequences on the surface roughness of three different nanocomposites and composite/ enamel and composite/ cementun interfaces. Nanomaterials 2020;10:1-14.
Yucci G Effect of Three Polishing Systems on the Surface Roughness of Microhybrid and Nano-filler Resins [Master’s thesis]. Universidad Nacional del Colombia; 2017. Available from: https://repositorio.unal.edu.co/handle/unal/62213
. [Last accessed on 2021 Jul 14].
Alfawaz Y Impact of polishing systems on the surface roughness and microhardness of nanocomposites. J Contemp Dent Pract 2017;18:647-51.
St-Pierre L, Martel C, Crépeau H, Vargas MA Influence of polishing systems on surface roughness of composite resins: Polishability of composite resins. Oper Dent 2019;44:E122-32.
Bansal K, Gupta S, Nikhil V, Jaiswal S, Jain A, Aggarwal N Effect of different finishing and polishing systems on the surface roughness of resin composite and enamel: An in vitro
profilometric and scanning electron microscopy study. Int J Appl Basic Med Res 2019;9:154-8.
Ramírez-Vargas GG, Medina y Mendoza JE, Aliaga-Mariñas AS, Ladera-Castañeda MI, Cervantes-Ganoza LA, Cayo-Rojas CF Effect of polishing on the surface microhardness of nanohybrid composite resins subjected to 35% hydrogen peroxide: An in vitro study. J Int Soc Prevent Communit Dent 2021;11:216-21.
[Figure 1], [Figure 2], [Figure 3], [Figure 4], [Figure 5], [Figure 6], [Figure 7], [Figure 8], [Figure 9]
[Table 1], [Table 2], [Table 3], [Table 4], [Table 5], [Table 6]
| Article Access Statistics|
| Viewed||111 |
| PDF Downloaded||5 |